#------------------------------------------------------------------------------
#$Date: 2016-02-21 02:03:34 +0200 (Sun, 21 Feb 2016) $
#$Revision: 176798 $
#$URL: svn://www.crystallography.net/cod/cif/2/23/96/2239626.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2239626
loop_
_publ_author_name
'Salloum, D.'
'Gougeon, P.'
'Gall, P.'
_publ_section_title
;
 Na~4.25~Mo₁₅S₁₉: a novel ternary reduced molybdenum sulfide
 containing Mo₆ and Mo₉ clusters
;
_journal_coeditor_code           RU2060
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i30
_journal_paper_doi               10.1107/S160053681401201X
_journal_volume                  70
_journal_year                    2014
_chemical_formula_iupac          'Na4.25 Mo15 S19'
_chemical_formula_sum            'Mo15 Na4.25 S19'
_chemical_formula_weight         2145.95
_chemical_name_systematic
;
Tetrasodium pentadecamolybdenum nonadecasulfide
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   9.53400(10)
_cell_length_b                   9.53400(10)
_cell_length_c                   18.9803(3)
_cell_measurement_reflns_used    16576
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.0
_cell_measurement_theta_min      2.15
_cell_volume                     1494.11(3)
_computing_cell_refinement       'COLLECT (Nonius, 1998)'
_computing_data_collection       'COLLECT (Nonius, 1998)'
_computing_data_reduction        'EvalCCD (Duisenberg, 1998)'
_computing_molecular_graphics    'DIAMOND (Bergerhoff, 1996)'
_computing_publication_material  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR97 (Altomare et al., 1999)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       'φ scans (κ = 0) + additional ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0848
_diffrn_reflns_av_sigmaI/netI    0.0306
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            16576
_diffrn_reflns_theta_full        29.99
_diffrn_reflns_theta_max         29.99
_diffrn_reflns_theta_min         2.15
_exptl_absorpt_coefficient_mu    7.443
_exptl_absorpt_correction_T_max  0.5914
_exptl_absorpt_correction_T_min  0.3631
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(de Meulenaar & Tompa, 1965)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.770
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'multi-faceted crystal'
_exptl_crystal_F_000             1962
_exptl_crystal_size_max          0.180
_exptl_crystal_size_mid          0.141
_exptl_crystal_size_min          0.080
_refine_diff_density_max         1.508
_refine_diff_density_min         -1.851
_refine_ls_extinction_coef       0.00266(19)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 2008)'
_refine_ls_goodness_of_fit_ref   1.130
_refine_ls_matrix_type           full
_refine_ls_number_parameters     66
_refine_ls_number_reflns         1500
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.130
_refine_ls_R_factor_all          0.0354
_refine_ls_R_factor_gt           0.0304
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0337P)²+5.1576P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0755
_refine_ls_wR_factor_ref         0.0787
_reflns_number_gt                1322
_reflns_number_total             1500
_reflns_threshold_expression     I>2sigma(I)
_cod_data_source_file            ru2060sup1.cf
_cod_data_source_block           I
_cod_database_code               2239626
_cod_database_fobs_code          2239626
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z-1/2'
'-y, x-y, -z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Mo Mo1 0.84424(3) 0.01344(3) -0.058496(18) 0.01072(12) Uani d . 1 1
Mo Mo2 0.50077(4) -0.18303(4) 0.131678(19) 0.01177(12) Uani d . 1 1
Mo Mo3 0.34797(5) -0.16448(5) 0.2500 0.01301(13) Uani d S 1 2
S S1 0.71650(10) 0.02755(11) 0.05118(5) 0.01268(18) Uani d . 1 1
S S2 0.36949(11) -0.01601(11) 0.13948(5) 0.01344(19) Uani d . 1 1
S S3 0.05126(16) -0.30754(17) 0.2500 0.0171(3) Uani d S 1 2
S S4 0.0000 0.0000 -0.15617(9) 0.0184(3) Uani d S 1 3
S S5 0.3333 -0.3333 0.03365(9) 0.0156(3) Uani d S 1 3
Na Na2 0.7703(5) -0.0623(4) -0.2500 0.0283(12) Uani d SP 0.751(12) 2
Na Na1 0.3333 -0.3333 -0.1085(3) 0.0789(17) Uani d S 1 3
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
S4 Mo1 S1 1_655 . 171.81(4)
S4 Mo1 S1 1_655 10_545 90.83(2)
S1 Mo1 S1 . 10_545 89.17(2)
S4 Mo1 S1 1_655 9_665 90.20(2)
S1 Mo1 S1 . 9_665 88.56(2)
S1 Mo1 S1 10_545 9_665 171.12(4)
S4 Mo1 S2 1_655 7_655 93.04(4)
S1 Mo1 S2 . 7_655 95.15(3)
S1 Mo1 S2 10_545 7_655 91.20(3)
S1 Mo1 S2 9_665 7_655 97.55(3)
S4 Mo1 Mo1 1_655 4_765 56.21(2)
S1 Mo1 Mo1 . 4_765 116.82(2)
S1 Mo1 Mo1 10_545 4_765 117.37(2)
S1 Mo1 Mo1 9_665 4_765 56.53(2)
S2 Mo1 Mo1 7_655 4_765 135.73(2)
S4 Mo1 Mo1 1_655 3_645 56.21(2)
S1 Mo1 Mo1 . 3_645 117.46(2)
S1 Mo1 Mo1 10_545 3_645 57.48(2)
S1 Mo1 Mo1 9_665 3_645 116.43(2)
S2 Mo1 Mo1 7_655 3_645 131.85(2)
Mo1 Mo1 Mo1 4_765 3_645 60.0
S4 Mo1 Mo1 1_655 9_665 116.37(2)
S1 Mo1 Mo1 . 9_665 56.60(2)
S1 Mo1 Mo1 10_545 9_665 115.84(3)
S1 Mo1 Mo1 9_665 9_665 56.08(2)
S2 Mo1 Mo1 7_655 9_665 138.14(2)
Mo1 Mo1 Mo1 4_765 9_665 60.241(8)
Mo1 Mo1 Mo1 3_645 9_665 90.0
S4 Mo1 Mo1 1_655 10_545 116.37(2)
S1 Mo1 Mo1 . 10_545 57.27(2)
S1 Mo1 Mo1 10_545 10_545 56.34(2)
S1 Mo1 Mo1 9_665 10_545 115.54(3)
S2 Mo1 Mo1 7_655 10_545 134.12(2)
Mo1 Mo1 Mo1 4_765 10_545 90.0
Mo1 Mo1 Mo1 3_645 10_545 60.241(8)
Mo1 Mo1 Mo1 9_665 10_545 59.518(16)
S4 Mo1 Na2 1_655 . 45.53(6)
S1 Mo1 Na2 . . 142.51(6)
S1 Mo1 Na2 10_545 . 83.36(6)
S1 Mo1 Na2 9_665 . 103.55(6)
S2 Mo1 Na2 7_655 . 48.59(6)
Mo1 Mo1 Na2 4_765 . 99.04(6)
Mo1 Mo1 Na2 3_645 . 88.97(5)
Mo1 Mo1 Na2 9_665 . 156.07(6)
Mo1 Mo1 Na2 10_545 . 137.75(5)
S5 Mo2 S2 . . 91.79(2)
S5 Mo2 S2 . 4_655 90.96(2)
S2 Mo2 S2 . 4_655 172.09(4)
S5 Mo2 S1 . . 92.26(3)
S2 Mo2 S1 . . 89.86(3)
S2 Mo2 S1 4_655 . 97.44(3)
S5 Mo2 S3 . 4_655 170.70(4)
S2 Mo2 S3 . 4_655 86.62(4)
S2 Mo2 S3 4_655 4_655 89.47(4)
S1 Mo2 S3 . 4_655 96.89(3)
S5 Mo2 Mo2 . 4_655 56.76(2)
S2 Mo2 Mo2 . 4_655 118.56(2)
S2 Mo2 Mo2 4_655 4_655 57.44(2)
S1 Mo2 Mo2 . 4_655 136.00(2)
S3 Mo2 Mo2 4_655 4_655 116.29(3)
S5 Mo2 Mo2 . 3_545 56.76(2)
S2 Mo2 Mo2 . 3_545 58.68(2)
S2 Mo2 Mo2 4_655 3_545 117.32(2)
S1 Mo2 Mo2 . 3_545 131.42(2)
S3 Mo2 Mo2 4_655 3_545 115.08(3)
Mo2 Mo2 Mo2 4_655 3_545 60.0
S5 Mo2 Mo3 . 4_655 118.14(2)
S2 Mo2 Mo3 . 4_655 115.63(3)
S2 Mo2 Mo3 4_655 4_655 56.66(2)
S1 Mo2 Mo3 . 4_655 137.83(3)
S3 Mo2 Mo3 4_655 4_655 54.99(3)
Mo2 Mo2 Mo3 4_655 4_655 61.444(11)
Mo2 Mo2 Mo3 3_545 4_655 90.670(10)
S5 Mo2 Mo3 . . 117.29(2)
S2 Mo2 Mo3 . . 56.69(2)
S2 Mo2 Mo3 4_655 . 115.55(3)
S1 Mo2 Mo3 . . 133.65(3)
S3 Mo2 Mo3 4_655 . 54.52(3)
Mo2 Mo2 Mo3 4_655 . 90.184(10)
Mo2 Mo2 Mo3 3_545 . 60.600(11)
Mo3 Mo2 Mo3 4_655 . 58.940(16)
S3 Mo3 S3 4_655 . 173.69(4)
S3 Mo3 S2 4_655 8_556 89.88(3)
S3 Mo3 S2 . 8_556 93.48(3)
S3 Mo3 S2 4_655 . 89.88(3)
S3 Mo3 S2 . . 93.48(3)
S2 Mo3 S2 8_556 . 115.45(4)
S3 Mo3 Mo3 4_655 3_545 117.00(4)
S3 Mo3 Mo3 . 3_545 56.69(4)
S2 Mo3 Mo3 8_556 3_545 118.47(2)
S2 Mo3 Mo3 . 3_545 118.47(2)
S3 Mo3 Mo3 4_655 4_655 57.00(4)
S3 Mo3 Mo3 . 4_655 116.69(4)
S2 Mo3 Mo3 8_556 4_655 116.54(2)
S2 Mo3 Mo3 . 4_655 116.54(2)
Mo3 Mo3 Mo3 3_545 4_655 60.0
S3 Mo3 Mo2 4_655 3_545 117.827(15)
S3 Mo3 Mo2 . 3_545 60.149(14)
S2 Mo3 Mo2 8_556 3_545 150.01(3)
S2 Mo3 Mo2 . 3_545 57.58(2)
Mo3 Mo3 Mo2 3_545 3_545 60.944(12)
Mo3 Mo3 Mo2 4_655 3_545 89.804(10)
S3 Mo3 Mo2 4_655 12_546 117.827(15)
S3 Mo3 Mo2 . 12_546 60.149(14)
S2 Mo3 Mo2 8_556 12_546 57.58(2)
S2 Mo3 Mo2 . 12_546 150.01(3)
Mo3 Mo3 Mo2 3_545 12_546 60.944(12)
Mo3 Mo3 Mo2 4_655 12_546 89.804(10)
Mo2 Mo3 Mo2 3_545 12_546 112.05(2)
S3 Mo3 Mo2 4_655 8_556 59.911(14)
S3 Mo3 Mo2 . 8_556 117.957(16)
S2 Mo3 Mo2 8_556 8_556 56.42(2)
S2 Mo3 Mo2 . 8_556 146.91(3)
Mo3 Mo3 Mo2 3_545 8_556 89.333(10)
Mo3 Mo3 Mo2 4_655 8_556 60.116(12)
Mo2 Mo3 Mo2 3_545 8_556 146.475(18)
Mo2 Mo3 Mo2 12_546 8_556 57.956(12)
S3 Mo3 Mo2 4_655 . 59.911(14)
S3 Mo3 Mo2 . . 117.957(16)
S2 Mo3 Mo2 8_556 . 146.91(3)
S2 Mo3 Mo2 . . 56.42(2)
Mo3 Mo3 Mo2 3_545 . 89.333(10)
Mo3 Mo3 Mo2 4_655 . 60.116(12)
Mo2 Mo3 Mo2 3_545 . 57.956(12)
Mo2 Mo3 Mo2 12_546 . 146.475(18)
Mo2 Mo3 Mo2 8_556 . 110.679(19)
S3 Mo3 Na2 4_655 7_655 117.20(8)
S3 Mo3 Na2 . 7_655 69.11(8)
S2 Mo3 Na2 8_556 7_655 61.70(3)
S2 Mo3 Na2 . 7_655 61.70(3)
Mo3 Mo3 Na2 3_545 7_655 125.80(8)
Mo3 Mo3 Na2 4_655 7_655 174.20(8)
Mo2 Mo3 Na2 3_545 7_655 93.43(4)
Mo2 Mo3 Na2 12_546 7_655 93.43(4)
Mo2 Mo3 Na2 8_556 7_655 117.90(3)
Mo2 Mo3 Na2 . 7_655 117.90(3)
Mo1 S1 Mo1 . 9_665 67.06(3)
Mo1 S1 Mo1 . 10_545 66.65(3)
Mo1 S1 Mo1 9_665 10_545 65.99(3)
Mo1 S1 Mo2 . . 134.06(4)
Mo1 S1 Mo2 9_665 . 130.92(4)
Mo1 S1 Mo2 10_545 . 82.94(3)
Mo1 S1 Na1 . 7_655 127.79(8)
Mo1 S1 Na1 9_665 7_655 97.39(3)
Mo1 S1 Na1 10_545 7_655 153.45(7)
Mo2 S1 Na1 . 7_655 94.64(6)
Mo2 S2 Mo3 . . 66.88(3)
Mo2 S2 Mo2 . 3_545 63.88(2)
Mo3 S2 Mo2 . 3_545 65.76(2)
Mo2 S2 Mo1 . 7_655 129.13(4)
Mo3 S2 Mo1 . 7_655 132.33(4)
Mo2 S2 Mo1 3_545 7_655 82.07(3)
Mo2 S2 Na2 . 7_655 133.09(7)
Mo3 S2 Na2 . 7_655 66.52(6)
Mo2 S2 Na2 3_545 7_655 100.94(8)
Mo1 S2 Na2 7_655 7_655 87.68(6)
Mo2 S2 Na1 . 7_655 101.03(3)
Mo3 S2 Na1 . 7_655 122.15(9)
Mo2 S2 Na1 3_545 7_655 160.14(7)
Mo1 S2 Na1 7_655 7_655 100.15(7)
Na2 S2 Na1 7_655 7_655 98.88(10)
Mo3 S3 Mo3 3_545 . 66.31(4)
Mo3 S3 Na2 3_545 10_445 157.19(11)
Mo3 S3 Na2 . 10_445 136.50(11)
Mo3 S3 Mo2 3_545 12_546 65.57(3)
Mo3 S3 Mo2 . 12_546 64.86(3)
Na2 S3 Mo2 10_445 12_546 119.39(3)
Mo3 S3 Mo2 3_545 3_545 65.57(3)
Mo3 S3 Mo2 . 3_545 64.86(3)
Na2 S3 Mo2 10_445 3_545 119.39(3)
Mo2 S3 Mo2 12_546 3_545 119.89(5)
Mo3 S3 Na2 3_545 7_655 128.66(8)
Mo3 S3 Na2 . 7_655 62.35(7)
Na2 S3 Na2 10_445 7_655 74.15(16)
Mo2 S3 Na2 12_546 7_655 92.16(5)
Mo2 S3 Na2 3_545 7_655 92.16(5)
Mo1 S4 Mo1 4_665 1_455 67.58(5)
Mo1 S4 Mo1 4_665 3_545 67.58(5)
Mo1 S4 Mo1 1_455 3_545 67.58(5)
Mo1 S4 Na2 4_665 1_455 151.15(7)
Mo1 S4 Na2 1_455 1_455 93.82(5)
Mo1 S4 Na2 3_545 1_455 127.12(7)
Mo1 S4 Na2 4_665 3_545 127.12(7)
Mo1 S4 Na2 1_455 3_545 151.15(7)
Mo1 S4 Na2 3_545 3_545 93.82(5)
Na2 S4 Na2 1_455 3_545 79.75(9)
Mo1 S4 Na2 4_665 4_665 93.82(5)
Mo1 S4 Na2 1_455 4_665 127.12(7)
Mo1 S4 Na2 3_545 4_665 151.15(7)
Na2 S4 Na2 1_455 4_665 79.75(9)
Na2 S4 Na2 3_545 4_665 79.75(9)
Mo2 S5 Mo2 3_545 . 66.48(4)
Mo2 S5 Mo2 3_545 4_655 66.48(4)
Mo2 S5 Mo2 . 4_655 66.48(4)
Mo2 S5 Na1 3_545 . 140.73(3)
Mo2 S5 Na1 . . 140.73(3)
Mo2 S5 Na1 4_655 . 140.73(3)
S3 Na2 S4 9_655 1_655 89.92(9)
S3 Na2 S4 9_655 8_655 89.92(9)
S4 Na2 S4 1_655 8_655 84.49(12)
S3 Na2 S2 9_655 2_654 112.74(10)
S4 Na2 S2 1_655 2_654 154.21(15)
S4 Na2 S2 8_655 2_654 83.46(4)
S3 Na2 S2 9_655 7_655 112.74(10)
S4 Na2 S2 1_655 7_655 83.46(4)
S4 Na2 S2 8_655 7_655 154.21(15)
S2 Na2 S2 2_654 7_655 97.94(11)
S3 Na2 Mo3 9_655 7_655 145.61(16)
S4 Na2 Mo3 1_655 7_655 114.79(9)
S4 Na2 Mo3 8_655 7_655 114.79(9)
S2 Na2 Mo3 2_654 7_655 51.78(6)
S2 Na2 Mo3 7_655 7_655 51.78(6)
S3 Na2 S3 9_655 7_655 165.85(15)
S4 Na2 S3 1_655 7_655 79.65(9)
S4 Na2 S3 8_655 7_655 79.65(9)
S2 Na2 S3 2_654 7_655 75.81(8)
S2 Na2 S3 7_655 7_655 75.81(8)
Mo3 Na2 S3 7_655 7_655 48.54(6)
S3 Na2 Na2 9_655 4_765 119.90(13)
S4 Na2 Na2 1_655 4_765 50.13(5)
S4 Na2 Na2 8_655 4_765 50.13(5)
S2 Na2 Na2 2_654 4_765 105.50(12)
S2 Na2 Na2 7_655 4_765 105.50(12)
Mo3 Na2 Na2 7_655 4_765 94.49(15)
S3 Na2 Na2 7_655 4_765 45.95(11)
S3 Na2 Na2 9_655 3_645 59.90(13)
S4 Na2 Na2 1_655 3_645 50.13(5)
S4 Na2 Na2 8_655 3_645 50.13(5)
S2 Na2 Na2 2_654 3_645 130.76(6)
S2 Na2 Na2 7_655 3_645 130.76(6)
Mo3 Na2 Na2 7_655 3_645 154.49(15)
S3 Na2 Na2 7_655 3_645 105.95(11)
Na2 Na2 Na2 4_765 3_645 60.0
S3 Na2 Mo1 9_655 . 97.96(5)
S4 Na2 Mo1 1_655 . 40.65(3)
S4 Na2 Mo1 8_655 . 124.10(12)
S2 Na2 Mo1 2_654 . 139.27(11)
S2 Na2 Mo1 7_655 . 43.72(2)
Mo3 Na2 Mo1 7_655 . 87.79(5)
S3 Na2 Mo1 7_655 . 80.39(5)
Na2 Na2 Mo1 4_765 . 79.33(6)
Na2 Na2 Mo1 3_645 . 87.34(5)
S3 Na2 Mo1 9_655 8 97.96(5)
S4 Na2 Mo1 1_655 8 124.10(12)
S4 Na2 Mo1 8_655 8 40.65(3)
S2 Na2 Mo1 2_654 8 43.72(2)
S2 Na2 Mo1 7_655 8 139.27(11)
Mo3 Na2 Mo1 7_655 8 87.79(5)
S3 Na2 Mo1 7_655 8 80.39(5)
Na2 Na2 Mo1 4_765 8 79.33(6)
Na2 Na2 Mo1 3_645 8 87.34(5)
Mo1 Na2 Mo1 . 8 157.78(11)
S5 Na1 S2 . 9 100.69(9)
S5 Na1 S2 . 7_655 100.69(9)
S2 Na1 S2 9 7_655 116.64(6)
S5 Na1 S2 . 10_545 100.69(9)
S2 Na1 S2 9 10_545 116.64(6)
S2 Na1 S2 7_655 10_545 116.64(6)
S5 Na1 S1 . 7_655 71.10(8)
S2 Na1 S1 9 7_655 66.58(2)
S2 Na1 S1 7_655 7_655 65.67(2)
S2 Na1 S1 10_545 7_655 171.77(17)
S5 Na1 S1 . 9 71.10(8)
S2 Na1 S1 9 9 65.67(2)
S2 Na1 S1 7_655 9 171.77(17)
S2 Na1 S1 10_545 9 66.58(2)
S1 Na1 S1 7_655 9 110.03(8)
S5 Na1 S1 . 10_545 71.10(8)
S2 Na1 S1 9 10_545 171.77(17)
S2 Na1 S1 7_655 10_545 66.58(2)
S2 Na1 S1 10_545 10_545 65.67(2)
S1 Na1 S1 7_655 10_545 110.03(8)
S1 Na1 S1 9 10_545 110.03(8)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Mo1 S4 1_655 2.4184(14)
Mo1 S1 . 2.4492(10)
Mo1 S1 10_545 2.4565(9)
Mo1 S1 9_665 2.4830(9)
Mo1 S2 7_655 2.5624(10)
Mo1 Mo1 4_765 2.6900(5)
Mo1 Mo1 3_645 2.6900(5)
Mo1 Mo1 9_665 2.7098(6)
Mo1 Mo1 10_545 2.7098(6)
Mo1 Na2 . 3.7042(8)
Mo2 S5 . 2.4033(13)
Mo2 S2 . 2.4733(9)
Mo2 S2 4_655 2.5070(9)
Mo2 S1 . 2.5429(10)
Mo2 S3 4_655 2.5947(8)
Mo2 Mo2 4_655 2.6349(5)
Mo2 Mo2 3_545 2.6349(5)
Mo2 Mo3 4_655 2.7081(4)
Mo2 Mo3 . 2.7303(4)
Mo3 S3 4_655 2.4419(14)
Mo3 S3 . 2.4504(14)
Mo3 S2 8_556 2.4810(10)
Mo3 S2 . 2.4810(10)
Mo3 Mo3 3_545 2.6756(7)
Mo3 Mo3 4_655 2.6756(7)
Mo3 Mo2 3_545 2.7081(4)
Mo3 Mo2 12_546 2.7081(4)
Mo3 Mo2 8_556 2.7303(4)
Mo3 Na2 7_655 2.896(3)
S1 Mo1 9_665 2.4565(9)
S1 Mo1 10_545 2.4830(9)
S1 Na1 7_655 3.3609(19)
S2 Mo2 3_545 2.5070(9)
S2 Mo1 7_655 2.5624(10)
S2 Na2 7_655 2.781(2)
S2 Na1 7_655 3.1669(13)
S3 Mo3 3_545 2.4419(14)
S3 Na2 10_445 2.538(4)
S3 Mo2 12_546 2.5947(8)
S3 Mo2 3_545 2.5947(8)
S3 Na2 7_655 3.055(4)
S4 Mo1 4_665 2.4184(14)
S4 Mo1 1_455 2.4184(14)
S4 Mo1 3_545 2.4184(14)
S4 Na2 1_455 2.649(3)
S4 Na2 3_545 2.649(3)
S4 Na2 4_665 2.649(3)
S5 Mo2 3_545 2.4033(13)
S5 Mo2 4_655 2.4033(13)
S5 Na1 . 2.699(5)
Na2 S3 9_655 2.538(4)
Na2 S4 1_655 2.649(3)
Na2 S4 8_655 2.649(3)
Na2 S2 2_654 2.781(2)
Na2 S2 7_655 2.781(2)
Na2 Mo3 7_655 2.896(3)
Na2 S3 7_655 3.055(4)
Na2 Na2 4_765 3.397(6)
Na2 Na2 3_645 3.397(6)
Na2 Mo1 8 3.7042(8)
Na1 S2 9 3.1669(13)
Na1 S2 7_655 3.1669(13)
Na1 S2 10_545 3.1669(13)
Na1 S1 7_655 3.3609(19)
Na1 S1 9 3.3609(19)
Na1 S1 10_545 3.3609(19)
